By Authority Of THE UNITED STATES OF AMERICA
Legally Binding Document By the Authority Vested By Part 5 of the United States Code § 552(a) and Part 1 of the Code of Regulations § 51 the attached document has been duly INCORPORATED BY REFERENCE and shall be considered legally binding upon all citizens and residents of the United States of America. HEED THIS NOTICE: Criminal penalties may apply for noncompliance.
e Document Name:
ASTM D4268: Standard Test Method for Testing Fiber Ropes
33 CFR 164.74(a)(3)(i)
American Society for Testing and Materials
Official Incorporator: THE EXECUTIVE DIRECTOR
OFFICE OF THE FEDERAL REGISTER WASHINGTON, D.C.
Designation: D 4268 - 93
Standard Test Methods for
Testing Fiber Ropes 1 This standard is issued under the fixed designation D 4268; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year oflast revision. A number in parentheses indicates the year oflast reapproval. A superscript epsilon (€) indicates an editorial change since the last revision or reapproval.
1. Scope 1.1 These test methods specify procedures to determine diameter and circumference (Section 8), linear density (Section 14), breaking force (Section 21), and elongation (Sections 28 and 36» of fiber ropes except those ropes incorporating steel wire. (See MIL-STD-191) 1.2 The values stated in SI units are to be regarded as standard. The values provided in parentheses are provided for information purposes only. 1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. Additional precautions for these test methods are given in Section 5. 2. Referenced Documents
"2.1 ASTM Standards: D 76 Specification for Tensile Testing Machines for Textiles2 D 123 Terminology Relating to Textiles2 E 4 Practices for Force Verification of Test Machines 3 E 74 Practice for Calibration of Force Measuring Instruments for Verifying the Load Indication of Testing Machines3 2.2 Military Standard4 : MIL-STD-191 3. Terminology 3.1 Definitions: 3.1.1 braided rope, n-a cylindrically produced rope made by intertwining, maypole fashion, several to many strands according to a definite pattern with adjacent strands normally containing yarns of the opposite twist. 3.1.2 cycle length n-in braided rope, the, distance, parallel to the rope axis, of the strand to make one revolution around the rope. 22.214.171.124 Discussion-pick count is reported in picks per metre, picks per foot, picks per inch, etc. 3.1.3 pick count n-in braided rope, the number of strands rotating in one direction in one cycle length. 1 These test methods are under the jurisdiction of ASTM Committee D-13 on Textiles and are the direct responsibility of Subcommittee D 13.16 on Ropes and Cordage. , Current edition approved July 15, 1993. Published September 1993. Originally published as D 4268 - 83. Last previous edition D 4268 - 93. 2 Annual Book of ASTM Standards, Vol 07.01. 3 Annual Book of ASTM Standards, Vol 03.01. 4 Available from Standardization Documents Order Desk, Bldg. 4 Section D, 700 Robbins Ave., Philadelphia, PA 19111-5094, Attn: NPODS.
3.1.4 elongation, n-the ratio of the change in length of a rope during application of tension to the original length of the rope when new. 126.96.36.199 non-elastic elongation (NE) n-ofrope, elongation after cyclic tensioning the rope to a specified force for a specified number of cycles. 188.8.131.52 recoverable elongation (eE) n-of rope, elongation which may be reclaimed following a period of rope relaxation after the rope was cyclic tensioned. 184.108.40.206 residual elongation (RE) n-of rope, elongation after cyclic tensioning the rope to a specified force for a specified number of cycles and allowing the rope to relax for a specified period of time. 220.127.116.11 working elongation (WE) n-of rope, elongation' which is immediately recoverable when tension is removed from the rope. 18.104.22.168 total elongation (TE) n-of rope, the entire elongation at any given applied force. 3.1.5 extension, n-the ratio of the change in length of a rope during application of tension to the length of the rope immediately before application of that load. ' 3.1.6 jiber rope, n-a rope produced primarily from textile fibers. 3.1.7 jid, n-a wooden or hard plastic tapered tool used as an aid in rope splicing. 3.1. 7 hockle, n-in rope, a strand kink in a rope causing yarn displacement in the strand resulting in rope deformation and damage. ' 3.1.8 kink, n-in rope, an abrupt bend or loop in the rope which is the result of an unbalanced twist relationship in the rope structure. 3.1.9 plaited rope, n-rope made from eight strands arranged in four pairs in which one strand is placed adjacent to the second in each pair and in whiwas :'used.. ,Most "usedi topes;' do ,S1iffer ,a strength loss due.to damage\ fromabrasion,buts,:mislise due to mishanqlirig;Jmprdpel' ,storage' or over tensioning. It can be expected that strength loss will occur dependi,ng llgation . of newi.rqpe during its initi~\ tension application", , 'i), ,~
number 'of cycles'to the .prescribed applied force., When cOlldubting i this test, in conjunction with 'Br€aking~Force Testing, :i.that ,prescribed" number'oR'cycles is ten and that prescribed ~applied; force, is, 20 % of. the' 'estitnated breaking force ..·For'gth€t, testing,· the prescribed number of cycles and the applied force shall be as agreed upon by the purchaser and seller.: Apply the pFescribed numbet of tensioning cycles continuously.; .! "" " ; \ " : ' < 40;5 BefOre ithe:rlast of the 'prescribed humber of cycles, with the rop'e at the R6ferenee Tensionsrneasure the distance betw.een ,marks' ,at the, prescribed ,applied force. This is Distance, C. :; i., " ~ ,, 40.S On the last of the prescribed number of cycles, measure the-" disUmc'e between, marks at. the prescribed applied force. 11his is iDistance D. ,';", . . "40;6;rWhenithe last prescribed ,cycler1has decreased to the Reference Force, 'again; m'easure' the~distance between inarks at this Reference Force. This is Distance Ei :, · .40.7 'Immecliately ,after :distance E -is determined, reduce t€nsion to Hi and leave the rope iIi a relaxed state (0 tension condition) for' 30 plus or minus, min. After the relaxation time, reapply the Reference Force and remeasure the distance between the marks'. This is distance F.
35. Precision and Bias 3S.1 Precision-Th~ precision of the procedllre in Test Methods D 4268 for detenniriing per6eht~ge ~Iong~tion of a new rope speci:p1~n during its initial ~xposure' to ~ensionin:g is being establi~hed. It is anticipated 'that the intedaborat